DisciplinaUnidade de Reabilitação Integral do Aparelho Estomatognático511 materiais • 973 seguidores
during 14 days.13 Contamination in the media was verifi ed ev- ery 48 h by means of Gram staining. Carious dentine removal and restoration The soft and infected carious tissue was removed with #8 round tungsten carbide burs (KGSorensen, Barueri, SP, Brazil) in a slow-speed handpiece (Fig- ure 1H). The tactile sensation criterion with dental explorers and visual examination were used to iden- tify the caries-affected dentin.1 Immediately after, Adper Scotchbond Multi-Purpose (3M-ESPE, St. Paul, MN, USA) was applied in accordance with the manufacturer\u2019s instructions (Table 1) and the bonded surfaces were coupled with a hybrid resin composite (Filtek Z250, 3M-ESPE, St. Paul, MN, USA lot1370A1) that was applied in 2-mm-thick increments and polymerized in a quartz-tungsten- halogen light-curing unit at 700 mW/cm2 (Tri-Light, 3M-ESPE, St. Paul, MN, USA) to form 4-mm-thick cores. Each increment was light-cured for 20 s. The teeth with composite build-ups were stored in Figure 1 - (A) Section perpendicular to the long axis of the tooth at 7 mm from the amelodentinal junction. (B) Flattened exposed dentin surface. (C) Samples painted with acid-resistant nail varnish, leaving 14.4 mm² of dentin surface area to be exposed to artificial caries development. (D) Samples fixed with orthodontic wires on the lids of glass container vessels. (E) Sterilization. (F) Inoculation of medium with Streptococcus mutans cultures. (G) Artificial caries development. The samples were transferred into fresh media every 48 h. (H) Soft and infected carious tissue removal with round tungsten carbide burs. (I) Res- toration. (J) Sterilization. (K) Cross-section performed perpendicularly to the restoration. (L) Beams obtained after the cutting procedures. (M) Specimen broken after microtensile testing. AA FF SterilizationSterilization EEDDCCBB MM LLKKIIHHGG JJ SterilizationSterilization Influence of sterilization method on the bond strength of caries-affected dentin Braz Oral Res 2009;23(1):11-614 distilled water at 37°C for 24 h (Figure 1I). After complete restoration, the specimens were sterilized again, in accordance with the method of each group, in the same manner reported previously (Figure 1J). Microtensile bond testing Each specimen was cross-sectioned perpendicu- larly to the resin-dentin interface with a slow-speed saw (Isomet, Buehler Ltd., Lake Bluff, IL, USA) under water cooling, yielding square beams of ap- proximately 1 mm2, in accordance with the non- trimming version of the microtensile bond test re- ported by Shono et al.15 (1999) (Figure 1K). Beams at specimen peripheries were discarded, yielding 10- 12 bonded beams per tooth (Figure 1L). Before bond-testing, the exact beam dimensions were measured to the nearest 0.01 mm with a digital caliper (Starret 727-6/150; Starret, Itu, SP, Brazil) to calculate bond strength, which was expressed in MPa. The beams were stressed to failure under ten- sion in a Bencor Multi-T device (Danville Engineer- ing, San Ramon, CA, USA) in a universal testing machine (Instron model 4411; Canton, MA, USA) at a crosshead speed of 0.5 mm/min (Figure 1M). The failure mode of each specimen was deter- mined under a stereomicroscope (Meiji EMZ-TR, Meiji Techno Co. Ltd., Tokyo, Japan) at x60 magni- fi cation and designated as an adhesive, mixed or co- hesive failure in either adhesive or resin composite. Statistical analysis The data were analyzed by the Mann-Whitney Test to examine the effect of sterilization method on bonding strength. Statistical signifi cance was set at \u3b1 = 0.05. Results Statistical analysis of the bond strength data de- rived for both methods of sterilization before arti- fi cial caries development and after complete resto- ration showed that the microtensile bond strengths of caries-affected dentin/resin were affected by the method used for sterilization (p < 0.05) (Table 2). Specimens sterilized with gamma-rays before artifi cial caries development and after complete restoration (G) exhibited signifi cantly higher bond strengths than specimens sterilized with steam auto- clave before and after (A). Group G showed higher bond strength values than group AG, but neither of them were statistically different from the control group (no sterilization \u2013 NE), with p = 0.06 and p = 0.79, respectively (Table 2). The failure mode obtained in group A was 75% mixed, 8.4% adhesive, and 16.6% cohesive in the Composition Mode of application Acid Conditioner: 37% Phosphoric acid (Batch:7523 5FB) Apply Acid Conditioner on dentin for 15 s, rinse for 15 s, dry gently for 2 s. Leave moist. Primer: water, ethanol, HEMAa, copolymer of polyalkanoic acid (Batch: 3008) Apply Primer to dentin. Dry gently for 5 s. Adhesive: BisGMAb, HEMA, dimethacrylate, initiators (Batch: 7583) Apply Adhesive to dentin. Light cure for 10 s. a: hydroxyethyl methacrylate. b: bisphenol A diglycidyl methacrylate. Table 1 - Composition and mode of application of the total etch adhesive system used in this study (Adper Scotchbond Multi-Purpose \u2013 3M-ESPE). Treatment Microtensile Bond Strength* No-sterilization (NE) 17.5 ± 10.8 (36)a, c Gamma-rays (G) 22.7 ± 11.3 (34)a Steam autoclave (A) 6.3 ± 4.4 (12)b Steam autoclave + Gamma-rays (AG) 16.3 ± 9.0 (33)c * Values are presented as mean ± standard deviation in MPa. Groups with the same superscripts are not statistically different (p > 0.05). The numbers of specimen beams tested are enclosed in parentheses. Table 2 - Microtensile bond strengths of the Adper Scotchbond Multi-Purpose adhesive system to caries-affected dentin in which sterilization methods were applied before artificial caries development and after complete restoration. Carvalho FG, Gonçalves LS, Carlo HL, Soares CJ, Correr-Sobrinho L, Puppin-Rontani RM Braz Oral Res 2009;23(1):11-6 15 adhesive. In group NE, the failure mode was 68% mixed, 4% adhesive, and 24% cohesive in the ad- hesive; and 4% cohesive in the resin. In group G, it was 70.6% mixed, and 29.4% cohesive in the adhe- sive. In group AG, it was 57.6% mixed, 39.4% cohe- sive in the adhesive, and 3% adhesive. Discussion The null hypothesis was not accepted since the sterilization method affected the bond strength of the caries-affected dentin, when used before artifi - cial caries development to produce artifi cial caries- affected dentin, and after complete restoration, in order to simulate secondary caries formation. The dose of gamma irradiation recommended for medical industry products is 25 kGy.16 However, the present study used a 14.5 kGy dose and it was able to sterilize without jeopardizing bond strength. Likewise, Rodrigues et al.12 (2005) demonstrated that a 14.5 kGy dose sterilized dental enamel blocks and no microbial growth was observed. The physi- cal and mechanical properties of the material are dose-dependent,17 thus, the lower the dose used for material sterilization (with no microbial growth), the less the alteration of their properties. Specimens sterilized with gamma-rays before ar- tifi cial caries development and after complete resto- ration exhibited signifi cantly higher bond strengths than the specimens sterilized with steam autoclave before and after. Although there are no investiga- tions about the effect of sterilization method on bond strength of dentin after restoration, the lower bond strength values in group A can be due to alter- ation in the dentin structure caused by steam auto- claving. FTIR spectra have demonstrated a change in the mineral component of dentin discs after au- toclave sterilization.7 Furthermore, an elevated tem- perature and high level of moisture were detrimental to adhesion, favoring water sorption, leaching resin components, disrupting polymer interchain hydro- gen bonds, causing a plasticization effect.18,19 These factors probably explain why several beams were debonded at the resin/dentine interface during the cross-sectioning of Group A beams.